Access the full text.
Sign up today, get DeepDyve free for 14 days.
Nardeep Kumar, S. Najmaei, Q. Cui, F. Ceballos, P. Ajayan, J. Lou, Hui Zhao (2013)
Second harmonic microscopy of monolayer MoS 2Physical Review B, 87
A. Splendiani, Liangyan Sun, Yuanbo Zhang, Tianshu Li, Jonghwan Kim, C. Chim, G. Galli, Feng Wang (2010)
Emerging photoluminescence in monolayer MoS2.Nano letters, 10 4
Shi-ning Zhu, Yong‐yuan Zhu, N. Ming (1997)
Quasi-phase-matched third-harmonic generation in a quasi-periodic optical superlatticeScience, 278
H. Rostami, M. Polini (2016)
Theory of third-harmonic generation in graphene: A diagrammatic approachPhysical Review B, 93
Hanzhe Liu, Yilei Li, Y. You, S. Ghimire, T. Heinz, D. Reis (2016)
High-harmonic generation from an atomically thin semiconductorNature Physics, 13
E. Hendry, P. Hale, J. Moger, A. Savchenko, S. Mikhailov (2009)
Coherent nonlinear optical response of graphene.Physical review letters, 105 9
R. Minck, R. Terhune, C. Wang (1966)
Nonlinear optics.Applied optics, 5 10
Yilei Li, Y. Rao, K. Mak, Y. You, Shuyuan Wang, C. Dean, T. Heinz (2013)
Probing symmetry properties of few-layer MoS2 and h-BN by optical second-harmonic generation.Nano letters, 13 7
K. Kieu, R. Jones, N. Peyghambarian (2010)
Generation of Few-Cycle Pulses From an Amplified Carbon Nanotube Mode-Locked Fiber Laser SystemIEEE Photonics Technology Letters, 22
D. Qiu, Felipe Jornada, S. Louie (2013)
Optical spectrum of MoS2: many-body effects and diversity of exciton states.Physical review letters, 111 21
authors contributed to the manuscript. Additional information Supplementary Information
Sheneve Butler, S. Hollen, Linyou Cao, Yi Cui, J. Gupta, H. Gutiérrez, T. Heinz, S. Hong, Jiaxing Huang, A. Ismach, E. Johnston-Halperin, M. Kuno, Vladimir Plashnitsa, R. Robinson, R. Ruoff, S. Salahuddin, J. Shan, Li Shi, M. Spencer, M. Terrones, W. Windl, J. Goldberger (2013)
Progress, challenges, and opportunities in two-dimensional materials beyond graphene.ACS nano, 7 4
B. Radisavljevic, A. Radenović, J. Brivio, V. Giacometti, A. Kis (2011)
Single-layer MoS2 transistors.Nature nanotechnology, 6 3
A. Chin, O. Calderón, J. Kono (2001)
Extreme midinfrared nonlinear optics in semiconductors.Physical review letters, 86 15
Qing Wang, K. Kalantar-zadeh, A. Kis, J. Coleman, M. Strano (2012)
Electronics and optoelectronics of two-dimensional transition metal dichalcogenides.Nature nanotechnology, 7 11
A. Willner, S. Khaleghi, M. Chitgarha, O. Yilmaz (2014)
All-Optical Signal ProcessingJournal of Lightwave Technology, 32
F. Bonaccorso, Zhipei Sun (2014)
Solution processing of graphene, topological insulators and other 2d crystals for ultrafast photonicsOptical Materials Express, 4
H. Haug, S. Koch (1990)
Quantum Theory of the Optical and Electronic Properties of Semiconductors
A. Kuc, N. Zibouche, T. Heine (2011)
Influence of quantum confinement on the electronic structure of the transition metal sulfide T S 2Physical Review B, 83
F. Hipólito, T. Pedersen, V. Pereira (2016)
Nonlinear photocurrents in two-dimensional systems based on graphene and boron nitridePhysical Review B, 94
M. Gruning, C. Attaccalite (2013)
Second harmonic generation in h-BN and MoS2 monolayers: Role of electron-hole interactionPhysical Review B, 89
(2013)
Tight-binding model and directgap/indirect-gap transition in single-layer and multilayer MoS2
Nardeep Kumar, J. Kumar, Christian Gerstenkorn, Rui Wang, Hsin-Ying Chiu, A. Smirl, Hui Zhao (2013)
Third harmonic generation in graphene and few-layer graphite filmsPhysical Review B, 87
G. Eda, H. Yamaguchi, D. Voiry, T. Fujita, Mingwei Chen, M. Chhowalla (2011)
Photoluminescence from chemically exfoliated MoS2.Nano letters, 11 12
R. Woodward, R. Murray, C. Phelan, R. Oliveira, T. Runcorn, E. Kelleher, S. Li, E Oliveira, G. Fechine, G. Eda, C. Matos (2016)
Characterization of the second- and third-order nonlinear optical susceptibilities of monolayer MoS2 using multiphoton microscopy2D Materials, 4
K. Seyler, J. Schaibley, Pu Gong, P. Rivera, Aaron Jones, Sanfeng Wu, Jiaqiang Yan, D. Mandrus, W. Yao, Xiaodong Xu (2015)
Electrical control of second-harmonic generation in a WSe2 monolayer transistor.Nature nanotechnology, 10 5
D. Clark, V. Senthilkumar, C. Le, D. Weerawarne, B. Shim, J. Jang, J. Shim, J. Cho, Yumin Sim, M. Seong, S. Rhim, A. Freeman, K. Chung, Yong Kim (2014)
Strong optical nonlinearity of CVD-grown MoS 2 monolayer as probed by wavelength-dependent second-harmonic generationPhysical Review B, 90
H. Rostami, R. Asgari, F. Guinea (2015)
Edge modes in zigzag and armchair ribbons of monolayer MoS2Journal of Physics: Condensed Matter, 28
R. Nair, P. Blake, A. Grigorenko, K. Novoselov, T. Booth, T. Stauber, N. Peres, SUPARNA DUTTASINHA (2008)
Fine Structure Constant Defines Visual Transparency of GrapheneScience, 320
A. Neto, F. Guinea, N. Peres, K. Novoselov, SUPARNA DUTTASINHA (2007)
The electronic properties of grapheneReviews of Modern Physics, 81
William Reece, Russell Sobelt (2000)
Diagrammatic Approach to
C. Le, D. Clark, F. Ullah, V. Senthilkumar, J. Jang, Yumin Sim, M. Seong, K. Chung, Hyoyeol Park, Yong Kim (2016)
Nonlinear optical characteristics of monolayer MoSe2Annalen der Physik, 528
N. Gottschalk (2016)
Fundamentals Of Photonics
Carmen Palacios-Berraquero, M. Barbone, D. Kara, Xiaolong Chen, I. Goykhman, D. Yoon, A. Ott, Jan Beitner, Kenji Watanabe, T. Taniguchi, A. Ferrari, M. Atatüre (2016)
Atomically thin quantum light-emitting diodesNature Communications, 7
W. Zipfel, Rebecca Williams, W. Webb (2003)
Nonlinear magic: multiphoton microscopy in the biosciencesNature Biotechnology, 21
Rafael Roldán, M. L'opez-Sancho, F. Guinea, E. Cappelluti, J. Silva-Guillén, P. Ordejón (2014)
Momentum dependence of spin–orbit interaction effects in single-layer and multi-layer transition metal dichalcogenides2D Materials, 1
A. Säynätjoki, L. Karvonen, J. Riikonen, Wonjae Kim, S. Mehravar, R. Norwood, N. Peyghambarian, H. Lipsanen, K. Kieu (2013)
Rapid large-area multiphoton microscopy for characterization of graphene.ACS nano, 7 10
F. Zahid, Lei Liu, Y. Zhu, Jian Wang, Hong Guo (2013)
A generic tight-binding model for monolayer, bilayer and bulk MoS2AIP Advances, 3
K. Kieu, Jason Jones, N. Peyghambarian (2010)
High power femtosecond source near 1 micron based on an all-fiber Er-doped mode-locked laserCLEO: 2011 - Laser Science to Photonic Applications
C. Le, Daniel Clark, F. Ullah, Joon Jang, V. Senthilkumar, Yumin Sim, M. Seong, K. Chung, Ji Kim, Sungkyun Park, S. Rhim, Gyungtae Kim, Yong Kim (2017)
Impact of Selenium Doping on Resonant Second-Harmonic Generation in Monolayer MoS2ACS Photonics, 4
N. Broderick, R. Brătfălean, T. Monro, D. Richardson, C. Sterke (2002)
Temperature and wavelength tuning of second-, third-, and fourth-harmonic generation in a two-dimensional hexagonally poled nonlinear crystalJournal of The Optical Society of America B-optical Physics, 19
F. Bonaccorso, Z. Sun, T. Hasan, A. Ferrari (2010)
Graphene Photonics and Optoelectroncs
H. Rostami, R. Rold'an, E. Cappelluti, R. Asgari, F. Guinea (2015)
Theory of strain in single-layer transition metal dichalcogenidesPhysical Review B, 92
Rui Wang, H. Chien, J. Kumar, Nardeep Kumar, Hsin-Ying Chiu, Hui Zhao (2014)
Third-harmonic generation in ultrathin films of MoS2.ACS applied materials & interfaces, 6 1
M. Trolle, G. Seifert, T. Pedersen (2013)
Theory of excitonic second-harmonic generation in monolayer MoS 2Physical Review B, 89
O. Pfister, J. Wells, L. Hollberg, L. Zink, D. Baak, M. Levenson, W. Bosenberg (1997)
Continuous-wave frequency tripling and quadrupling by simultaneous three-wave mixings in periodically poled crystals: application to a two-step 1.19-10.71-microm frequency bridge.Optics letters, 22 16
(2012)
Introduction to Electrodynamics (Pearson
L. Chirolli, M. Polini, V. Giovannetti, A. Macdonald (2012)
Drude weight, cyclotron resonance, and the Dicke model of graphene cavity QED.Physical review letters, 109 26
G. Giuliani, G. Vignale (2005)
Quantum Theory of the Electron Liquid
Jisook Lee, K. Novoselov, H. Shin (2011)
Interaction between metal and graphene: dependence on the layer number of graphene.ACS nano, 5 1
M. Amani, D. Lien, D. Kiriya, Jun Xiao, A. Azcatl, Jiyoung Noh, S. Madhvapathy, R. Addou, Santosh Kc, M. Dubey, Kyeongjae Cho, R. Wallace, Si-Chen Lee, Jr-hau He, J. Ager, Xiang Zhang, E. Yablonovitch, A. Javey (2015)
Near-unity photoluminescence quantum yield in MoS2Science, 350
N. Alidoust, G. Bian, Su-Yang Xu, R. Sankar, M. Neupane, Chang Liu, I. Belopolski, D. Qu, J. Denlinger, F. Chou, M Hasan (2013)
Observation of monolayer valence band spin-orbit effect and induced quantum well states in MoX2Nature Communications, 5
R. Miller (1964)
OPTICAL SECOND HARMONIC GENERATION IN PIEZOELECTRIC CRYSTALSApplied Physics Letters, 5
N. Bhattacharya, E. Weiss (2012)
Second Harmonic Generation Imaging
L. Karvonen, A. Säynätjoki, S. Mehravar, R. Rodriguez, Susanne Hartmann, D. Zahn, S. Honkanen, R. Norwood, N. Peyghambarian, K. Kieu, H. Lipsanen, J. Riikonen (2015)
Investigation of Second- and Third-Harmonic Generation in Few-Layer Gallium Selenide by Multiphoton MicroscopyScientific Reports, 5
Xiaodong Xu, W. Yao, Di Xiao, T. Heinz (2014)
Spin and pseudospins in layered transition metal dichalcogenidesNature Physics, 10
A. Korm'anyos, V. Z'olyomi, N. Drummond, P. Rakyta, G. Burkard, V. Fal’ko (2013)
Monolayer MoS 2 : Trigonal warping, the Γ valley, and spin-orbit coupling effectsPhysical Review B, 88
T. Cheiwchanchamnangij, W. Lambrecht (2012)
Quasiparticle band structure calculation of monolayer, bilayer, and bulk MoS 2Physical Review B, 85
Jinluo Cheng, N. Vermeulen, J. Sipe (2014)
Third order optical nonlinearity of grapheneNew Journal of Physics, 16
Sanfeng Wu, Li Mao, Aaron Jones, W. Yao, Chuanwei Zhang, Xiaodong Xu (2012)
Quantum-enhanced tunable second-order optical nonlinearity in bilayer graphene.Nano letters, 12 4
(2016)
Ultra-strong nonlinear optical processes and trigonal warping in MoS$_2$ layers
Hongliang Shi, H. Pan, Yong-Wei Zhang, B. Yakobson (2012)
Quasiparticle band structures and optical properties of strained monolayer MoS 2 and WS 2Physical Review B, 87
M. Gibertini, F. Pellegrino, N. Marzari, M. Polini (2014)
Spin-resolved optical conductivity of two-dimensional group-VIB transition-metal dichalcogenidesPhysical Review B, 90
C. Casiraghi, A. Hartschuh, E. Lidorikis, H. Qian, H. Harutyunyan, T. Gokus, K. Novoselov, A. Ferrari (2007)
Rayleigh imaging of graphene and graphene layers.Nano letters, 7 9
Zhipei Sun, Amos Martinez, Feng Wang (2016)
Optical modulators with 2D layered materialsNature Photonics, 10
A. Ramasubramaniam (2012)
Large excitonic effects in monolayers of molybdenum and tungsten dichalcogenidesPhysical Review B, 86
F. Bonaccorso, A. Lombardo, T. Hasan, Zhipei Sun, L. Colombo, A. Ferrari (2012)
Production and processing of graphene and 2d crystalsMaterials Today, 15
Sung-Young Hong, J. Dadap, Nicholas Petrone, P. Yeh, J. Hone, R. Osgood (2013)
Optical Third-Harmonic Generation in GraphenePhysical Review X, 3
X. Zhang, W. Han, J. Wu, S. Milana, Y. Lu, Q. Li, A. Ferrari, P. Tan (2012)
Raman spectroscopy of shear and layer breathing modes in multilayer MoS2Physical Review B, 87
K. Novoselov, D. Jiang, F. Schedin, T. Booth, V. Khotkevich, S. Morozov, SUPARNA DUTTASINHA (2005)
Two-dimensional atomic crystals.Proceedings of the National Academy of Sciences of the United States of America, 102 30
Gang Wang, X. Marie, I. Gerber, T. Amand, D. Lagarde, L. Bouet, M. Vidal, A. Balocchi, B. Urbaszek (2014)
Giant enhancement of the optical second-harmonic emission of WSe(2) monolayers by laser excitation at exciton resonances.Physical review letters, 114 9
Di Xiao, Gui-Bin Liu, W. Feng, Xiaodong Xu, W. Yao (2011)
Coupled spin and valley physics in monolayers of MoS2 and other group-VI dichalcogenides.Physical review letters, 108 19
Thomas Tsang (1995)
Optical third-harmonic generation at interfaces.Physical review. A, Atomic, molecular, and optical physics, 52 5
F. Koppens, T. Mueller, P. Avouris, A. Ferrari, M. Vitiello, M. Polini (2014)
Photodetectors based on graphene, other two-dimensional materials and hybrid systems.Nature nanotechnology, 9 10
J Bhawalkar, G He, P Prasad (1997)
Nonlinear multiphoton processes in organic and polymeric materialsReports on Progress in Physics, 60
C. Janisch, Yuanxi Wang, Ding Ma, N. Mehta, A. Elías, N. Peréa-López, M. Terrones, V. Crespi, Zhiwen Liu (2014)
Extraordinary Second Harmonic Generation in Tungsten Disulfide MonolayersScientific Reports, 4
G. Eda, S. Maier (2013)
Two-dimensional crystals: managing light for optoelectronics.ACS nano, 7 7
S Jafari (2012)
Nonlinear optical response in gapped grapheneJournal of Physics: Condensed Matter, 24
S. Brun, T. Pedersen (2015)
Intense and tunable second-harmonic generation in biased bilayer graphenePhysical Review B, 91
H. Rostami, Ali Moghaddam, R. Asgari (2013)
Effective lattice Hamiltonian for monolayer MoS 2 : Tailoring electronic structure with perpendicular electric and magnetic fieldsPhysical Review B, 88
(1981)
Many-Particle Physics: Physics of Solids and Liquids
V. Margulis, E. Muryumin, E. Gaiduk (2013)
Optical second-harmonic generation from two-dimensional hexagonal crystals with broken space inversion symmetryJournal of Physics: Condensed Matter, 25
E. Kadantsev, P. Hawrylak (2012)
Electronic structure of a single MoS2 monolayerSolid State Communications, 152
D. Clark, C. Le, V. Senthilkumar, F. Ullah, H. Cho, Yumin Sim, M. Seong, K. Chung, Yong Kim, J. Jang (2015)
Near bandgap second-order nonlinear optical characteristics of MoS2 monolayer transferred on transparent substratesApplied Physics Letters, 107
R. Sundaram, Michael Engel, A. Lombardo, R. Krupke, A. Ferrari, P. Avouris, M. Steiner (2012)
Electroluminescence in single layer MoS2.Nano letters, 13 4
K. Mak, K. He, Changgu Lee, Gwan‐Hyoung Lee, J. Hone, T. Heinz, J. Shan (2012)
Tightly bound trions in monolayer MoS2.Nature materials, 12 3
P. Butcher, D. Cotter (1990)
The Elements of Nonlinear Optics: Preface
L. Malard, T. Alencar, A. Barboza, K. Mak, A. Paula (2013)
Observation of intense second harmonic generation from MoS 2 atomic crystalsPhysical Review B, 87
K. Mak, Changgu Lee, J. Hone, J. Shan, T. Heinz (2010)
Atomically thin MoS₂: a new direct-gap semiconductor.Physical review letters, 105 13
ONR NECom MURI, CIAN NSF ERC under Grant EEC-0812072, and TRIF Photonics funding from the state of Arizona and the Micronova
A. Ferrari, F. Bonaccorso, V. Fal’ko, K. Novoselov, S. Roche, P. Bøggild, S. Borini, F. Koppens, V. Palermo, N. Pugno, J. Garrido, R. Sordan, A. Bianco, L. Ballerini, M. Prato, E. Lidorikis, J. Kivioja, C. Marinelli, T. Ryhänen, A. Morpurgo, J. Coleman, V. Nicolosi, L. Colombo, A. Fert, M. García-Hernández, A. Bachtold, G. Schneider, F. Guinea, C. Dekker, M. Barbone, Zhipei Sun, C. Galiotis, A. Grigorenko, G. Konstantatos, A. Kis, M. Katsnelson, L. Vandersypen, Annick Loiseau, V. Morandi, D. Neumaier, E. Treossi, V. Pellegrini, M. Polini, A. Tredicucci, Gareth Williams, B. Hong, Jong-Hyun Ahn, Jong Kim, H. Zirath, B. Wees, H. Zant, L. Occhipinti, A. Matteo, I. Kinloch, T. Seyller, E. Quesnel, Xinliang Feng, K. Teo, N. Rupesinghe, P. Hakonen, Simon Neil, Quentin Tannock, T. Löfwander, J. Kinaret (2015)
Science and technology roadmap for graphene, related two-dimensional crystals, and hybrid systems.Nanoscale, 7 11
Kangpeng Wang, Jun Wang, Jintai Fan, M. Lotya, A. O’Neill, D. Fox, Yanyan Feng, Xiaoyan Zhang, B. Jiang, Quanzhong Zhao, Hongzhou Zhang, J. Coleman, Long Zhang, W. Blau (2013)
Ultrafast saturable absorption of two-dimensional MoS2 nanosheets.ACS nano, 7 10
ARTICLE DOI: 10.1038/s41467-017-00749-4 OPEN Ultra-strong nonlinear optical processes and trigonal warping in MoS layers 1,2 1 3 1 4 Antti Säynätjoki , Lasse Karvonen , Habib Rostami , Anton Autere , Soroush Mehravar , 5 4 5 1,2,4 1 Antonio Lombardo , Robert A. Norwood , Tawﬁque Hasan , Nasser Peyghambarian , Harri Lipsanen , 4 5 3 1 Khanh Kieu , Andrea C. Ferrari , Marco Polini & Zhipei Sun Nonlinear optical processes, such as harmonic generation, are of great interest for various applications, e.g., microscopy, therapy, and frequency conversion. However, high-order har- monic conversion is typically much less efﬁcient than low-order, due to the weak intrinsic response of the higher-order nonlinear processes. Here we report ultra-strong optical non- linearities in monolayer MoS (1L-MoS ): the third harmonic is 30 times stronger than the 2 2 second, and the fourth is comparable to the second. The third harmonic generation efﬁciency for 1L-MoS is approximately three times higher than that for graphene, which was reported (3) to have a large χ . We explain this by calculating the nonlinear response functions of 1L- MoS with a continuum-model Hamiltonian and quantum mechanical diagrammatic pertur- bation theory, highlighting the role of trigonal warping. A similar effect is expected in all other transition-metal dichalcogenides. Our results pave the way for efﬁcient harmonic generation based on layered materials for applications such as microscopy and imaging. 1 2 Department of Electronics and Nanoengineering, Aalto University, Tietotie 3, FI-02150 Espoo, Finland. Institute of Photonics, University of Eastern Finland, 3 4 Yliopistokatu 7, FI-80100 Joensuu, Finland. Istituto Italiano di Tecnologia, Graphene Labs, Via Morego 30, I-16163 Genova, Italy. College of Optical Sciences, University of Arizona, 1630 E University Blvd, Tucson, AZ 85721, USA. Cambridge Graphene Centre, University of Cambridge, Cambridge CB3 0FA, UK. Antti Säynätjoki, Lasse Karvonen and Habib Rostami contributed equally to this work. Correspondence and requests for materials should be addressed to Z.S. (email: zhipei.sun@aalto.ﬁ) NATURE COMMUNICATIONS 8: 893 DOI: 10.1038/s41467-017-00749-4 www.nature.com/naturecommunications 1 | | | ARTICLE NATURE COMMUNICATIONS | DOI: 10.1038/s41467-017-00749-4 onlinear optical phenomena can generate high-energy no second harmonic (SH) signal. On the other hand, MoS with photons by converting n = 2, 3, 4,… low-energy photons odd number of layers (ON) is non-centrosymmetric. SHG from 1L- 14–21 Ninto one high-energy photon. These are usually referred to MoS was reported by several groups . as second-, third-, and fourth-harmonic generation (SHG, THG, Here we present combined experimental and theoretical work 1 1, 2 and FHG) . Due to different selection rules , harmonic processes on nonlinear harmonic generation in 1L and few-layer (FL) MoS . are distinct from optically pumped laser phenomena (e.g., optically We report strong THG and FHG from 1L-MoS . THG is more pumped ampliﬁcation ), and other typical single-photon processes than one order of magnitude larger than SHG, while FHG has the (e.g., single-photon excited photoluminescence ), in which the same magnitude as SHG. This is surprising, since one normally energy of the generated photons is smaller than the pump photons. expects the intensity of nonlinear optical processes to decrease 1, 2 Multiphoton harmonic processes have been widely exploited for with n , with the SHG intensity much larger than that in THG various applications (e.g., all-optical signal processing in tele- and FHG, although even-order processes only exist in non-cen- 1, 4 5 6 communications ,medicine , and data storage ), as well as to trosymmetric materials. Our results show that this expectation is study various transitions forbidden under low-energy single-photon wrong in the case of 1L-MoS . At sufﬁciently low photon fre- 5, 6 excitation . The physical origin of these processes is the nonlinear quencies (in our experiments the photon energy of the pump is polarization induced by an electromagnetic ﬁeld E. This gives rise to 0.8 eV), SHG only probes the low-energy band structure of 1L- 22–29 higher harmonic components, the n-th harmonic component MoS . This is nearly rotationally invariant , but with correc- 1 n amplitude being proportional to |E| . Quantum mechanically, tions due to trigonal warping. It is because of these 23, 26, 27 1 1 higher-harmonic generation involves the annihilation of n pump corrections , fully compatible with the D space group , 3h photons and generation of a photon with n times the pump energy. but reducing the full rotational symmetry of the low-energy bands Because an n-th order nonlinear optical process requires n photons to a three-fold rotational symmetry ,thata ﬁnite amplitude of to be present simultaneously, the probability of higher-order pro- nonlinear harmonic processes can exist at low photon energies in cessesislower than that of lowerorder . Thus, higher-order pro- EN-MoS . The lack of spatial inversion symmetry is a necessary 7, 8 cesses are typically weaker and require higher pump intensities . but not sufﬁcient condition for the occurrence of SHG. A purely 30–33 Graphene and related materials are at the center of an ever- isotropic band structure gives a vanishing SHG signal , despite increasing research effort due to their unique and complementary some terms in the Hamiltonian explicitly breaking inversion 27, 34–37 properties, making them appealing for a wide range of photonic and symmetry . Terms proportional to the σ Pauli matrix 9–11 optoelectronic applications . Among these, semiconducting break inversion symmetry. Breaking the continuous rotational transition-metal dichalcogenides (TMDs) are of particular interest symmetry of isotropic models (e.g., by including trigonal warping) due to their direct bandgap when in monolayer (1L) form ,leading is required to obtain a non-zero second-order response in a two- to an increase in luminescence by a few orders of magnitude band system. In hexagonal lattices, trigonal warping is a deviation 12, 13 compared with the bulk material . 1L-MoS has a single layer of from purely isotropic bands that emerges as one moves away from 23, 26, 27, 36–38 Mo atoms sandwiched between two layers of S atoms in a trigonal the corners K and K′ of the Brillouin zone . Since the prismatic lattice. Therefore, in contrast to graphene, it is non-cen- lattice has a honeycomb structure, this distortion displays a three- 1 14 23, 26, 27, 36–38 trosymmetric and belongs to the space group D .The lack of fold rotational symmetry . We demonstrate that the 3h spatial inversion symmetry makes 1L-MoS an interesting material observed THG/SHG intensity ratio can be explained by quantum for nonlinear optics, since second-order nonlinear processes are mechanical calculations based on ﬁnite-temperature many-body 1 39 present only in non-centrosymmetric materials . However, when diagrammatic perturbation theory and low-energy continuum- stacked, MoS layers are arranged mirrored with respect to one model Hamiltonians that include trigonal warping . We conclude 14 14–18 another , therefore MoS with an even number of layers (EN) is that, similar to SHG , the THG process is sensitive to the 3 14 centrosymmetric and belongs to the D space group ,producing number of layers, their symmetry, relative orientation, as well as 3d ab 1g 2g 5L-MoS 1L 2L 2L 2L-MoS 1L 2L 1L 1L-MoS 360 380 400 420 440 20 µm 5L –1 Raman shift (cm ) Fig. 1 Optical image and Raman spectra of the MoS ﬂakes. a Optical micrograph with single-layer, bilayer, and ﬁve-layer areas marked by 1L, 2L, and 5L. b Raman spectra of the same sample 2 NATURE COMMUNICATIONS 8: 893 DOI: 10.1038/s41467-017-00749-4 www.nature.com/naturecommunications | | | Intensity (a.u.) PMT NATURE COMMUNICATIONS | DOI: 10.1038/s41467-017-00749-4 ARTICLE Collimator ab QWP VA SHG THG Galvo scanner Scans lens MLL Power (pW) Power (nW) 0 4.5 0 3.4 Dichroic mirror (562 nm) THG Tube lens Collection lens 520 nm BP filter 0.1 SHG 0.01 Dichroic mirror FHG PMT (870 nm) 1E–3 780 nm BP filter 1E–4 20X 1E–5 400 500 600 700 800 Wavelength (nm) Sample Fig. 3 Multiphoton images of MoS ﬂakes. a SHG and b THG map of the ﬂakes in Fig. 1a. c Optical spectrum of the nonlinear signal from 1L-MoS −2 with a peak irradiance ~30 GW cm Fig. 2 Schematic diagram of multiphoton microscope. MLL, linearly polarized mode-locked ﬁber laser. VA, variable attenuator. QWP, quarter- wave plate used to study the dependence of SHG and THG on the elliptical polarization of the pump light. BP ﬁlter, bandpass ﬁlter. PMT, and enables high signal-to-noise-ratio, even with acquisition time photomultiplier tube per pixel in the μs range. SHG and THG images of the MoS sample are shown in Fig. 3a, b. The SH photon energy is ~1.6 eV, lower than the 12, 13 bandgap of 1L-MoS . This is not unexpected, as harmonic the elliptical polarization of the excitation light. Similar effects are generation can occur when the harmonic energy is below expected for all other TMDs. This paves the way for the assembly 1, 47, 48 the bandgap . The SHG signal is generated in 1L-MoS , of heterostructures with tailored nonlinear optical properties. while 2L-MoS appears dark. As discussed above, the second- order nonlinear response is present in 1L-MoS , which is non- Results centrosymmetric. However, when stacked to form 2L-MoS , 14, 15 Samples. MoS ﬂakes are produced by micromechanical cleavage MoS layers are mirrored . Therefore, EN-MoS is centro- 2 2 14, 15 3 14, 15 (MC) of bulk MoS onto Si + 285 nm SiO . 1L-MoS and bilayer 2 2 2 symmetric , and belongs to the D space group , 3d (2L-MoS ) ﬂakes are identiﬁed by a combination of optical 2 producing no SHG signal. On the other hand, ON-MoS ﬂakes 41, 42 43 14, 15 contrast and Raman spectroscopy . Raman spectra are are non-centrosymmetric . acquired by a Renishaw micro-Raman spectrometer equipped We note that strong THG is detected compared with SHG, even with a 600 line/mm grating and coupled with an Ar ion laser at for 1L-MoS ,Fig. 3b. THG was previously reported for a 7L-MoS 2 2 18 49 514.5 nm. Figure 1a shows the MoS ﬂakes studied in this work 2 ﬂake , but here we see it down to 1L-MoS . Reference followed and their Raman signatures. A reference MC graphene sample is our work and reported THG and SHG from 1L-MoS , giving ð2Þ also prepared and placed on a similar substrate. effective bulk-like second- and third-order susceptibilities χ eff ð3Þ −11 −1 −19 2 −2 and χ of 2.9 × 10 mV and 2.4 × 10 m V , respectively. eff However, ref. did not provide a detailed explanation of the large SHG and THG charcterization. Nonlinear optical measurements THG signal compared to the SHG. Instead it assigned the large 44, 45 are carried out with the set-up shown in Fig. 2 . As excitation THG/SHG ratio to a possible enhancement of THG by the edge of source, we use an erbium-doped mode-locked ﬁber laser with a 51, 52 the B exciton. However, refs. demonstrated that SHG is 50 MHz repetition rate, maximum average power 60 mW, and enhanced only when the SHG wavelength overlaps the A or B pulse duration 150 fs, which yields an estimated pulse peak power excitons. A similar behavior is expected for THG. Thus, the of ~8 kW . The laser beam is scanned with a galvo mirror 49 53 explanationinref. may not be correct. Reference reported and focused on the sample using a microscope objective. The high-harmonic (>6th-order) generation in the non-perturbative back-scattered second and third harmonic signals are split into regime with mid-infrared (IR) excitation (0.3 eV), unlike our THG different branches using a dichroic mirror and then detected and FHG results with near-IR excitation (0.8 eV). We do not detect using photomultiplier tubes (PMTs). For two-channel detection, THG from the thickest areas of our ﬂake, with N > 30, as in ref. . the light is split into two PMTs using a dichroic mirror with The output spectrum in Fig. 3c further conﬁrms that we observe 562 nm cutoff. After the dichroic mirror, the detected wavelength both SHG and THG. Peaks for THG and SHG at 520 and 780 nm range can be further reﬁned using bandpass ﬁlters. The light can can be seen, as well as at 390 nm, corresponding to a four-photon also be directed to a spectrometer (OceanOptics QE Pro-FL). The process. This is detected only in 1L-MoS . Its intensity is ~5.5 times average power on the sample is kept between 10 and 28 mW with lower than SHG, and two orders of magnitude smaller than THG. a typical measurement time ~5 μs, which prevents sample damage NATURE COMMUNICATIONS 8: 893 DOI: 10.1038/s41467-017-00749-4 www.nature.com/naturecommunications 3 | | | Intensity (a.u.) ARTICLE NATURE COMMUNICATIONS | DOI: 10.1038/s41467-017-00749-4 (780 nm), below the band gap of 1L-MoS , therefore are not a 0.4 15 adsorbed, unlike the SHG signal in ref. . SHG Second- and third-order nonlinear susceptibilities. Based on 0.3 the measured SHG and THG intensities, we can estimate the (2) (3) (2) 10 nonlinear susceptibilities χ and χ . χ can be calculated from the measured average powers of the fundamental and SH signals 0.2 as follows : sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 5 ϵ cλ P RτðÞ n þ 1ðÞ n þ 1 0 2ω 2 1 ð2Þ ð1Þ χ ¼ ; 0.1 s 32N τ P ϕ 2 pump where τ is the pulse width, P is the average power of the pump incident fundamental (pump) beam, and P stands for 0 0 2ω 1 234 567 the generated SH beam power, R is the repetition rate, N = 0.5 Number of layers is the numerical aperture, λ = 780 nm is the SH wavelength, τ = τ = 150 fs are the pulse durations at fundamental and R pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 2 b 1 2 SH wavelengths, ϕ ¼ 8π jcos ρ ρ 1 ρ j ρ dρ ¼ 3:56 from ref. , and n ¼ n 1:45 are the refractive indexes of 1 2 the substrate at the wavelengths of the fundamental and SHG, respectively. The effective bulk-like second-order susceptibility of ð2Þ ð2Þ ð2Þ MoS ðχ Þ can be obtained from Eq. (1) with χ ¼ , where eff eff t MoS 10, 24 t ¼ 0:65 nm is the 1L-MoS thickness . We obtain the MoS 2 ð2Þ −1 effective second-order susceptibility χ 2:2 pmV for 1L- eff MoS . Reference reported a bulk-like second-order suscept- −1 ibility 29 pmV , which is ~10 times larger than here. However, −1 20, 52, 55 0.1 several other studies reported ~5 pmV for 1560 nm . ð2Þ Thus, our measured χ agrees well with earlier values measured eff with similar excitation wavelength. ð3Þ The third-order susceptibility χ can be estimated eff 0.5 1 1.5 2 by comparing the measured THG signal from MoS to that of Pump peak power on sample (kW) 1L-graphene (SLG): rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ t THG ð3Þ SLG MoS ð3Þ k a = 0.85 c 0 ð2Þ χ χ : SLG eff 64 t THG k a = 0.9 MoS SLG c 0 k a = 0.95 c 0 with t = 0.33 nm the SLG thickness, and THG and SLG SLG k a = 1.0 c 0 THG the measured signals from SLG and MoS , respectively. MoS 2 16 2 EXP. Our results show that THG from 1L-MoS is around three times (3) larger than THG , which indicates that χ of 1L-MoS is SLG 2 comparable to that of SLG, in the frequency range of our 4 ð3Þ 49, 56 experiments. Previous reports indicate that χ is SLG −17 −19 2 −2 (3) ~10 –10 m V . Thus, based on Eq. (2), χ of 1L-MoS is in the same range. This is remarkable, as SLG is known to have (3)56–59 18 (3) a large χ . Reference reported χ of 7L-MoS to be ð3Þ approximately three orders of magnitude smaller than χ of SLG 200 400 800 1800 ð3Þ 56 56 58 ref. . χ from ref. is much higher than other theoretical SLG P (W) 49 pump and experimental values. We believe that our measured ratio between 1L-MoS and SLG is more accurate, since we measured Fig. 4 Experimental and theoretical nonlinear optical processes in MoS . both materials at the same time under the same conditions. a SHG and THG intensities as functions of N. b Power dependence of We note that large discrepancies can be found in earlier reported SHG and THG in 1L-MoS . c Experimental and theoretical THG/SHG effective susceptibilities for layered materials (LM). For example, irradiance ratio as a function of P . Different theoretical curves refer to pump (3) pﬃﬃﬃ there is a approximately four orders of magnitude difference in χ different values of the ultra-violet cutoff k (in units of 1=a ¼ 3=a; where c 0 −15 2 −2 57 −19 2 −2 49 for SLG (~10 m V in ref. ;~10 m V in ref. ). There is a = 3.16 Å is the lattice constant of 1L-MoS ). Black dashed lines in panels (2) an approximately three orders of magnitude difference in χ a and b are a guide to the eye. The error bars in c account for experimental −7 −1 15 reported for 1L-MoS at 800 nm (e.g., ~10 mV in ref. ;and uncertainties −10 −1 17 ~10 mV in ref. ). Effective susceptibilities are well deﬁned only in three-dimensional materials, since their deﬁnition involves a polarization per unit volume . Therefore, given the large discre- SHG signals on areas with N = 3, 5, 7 have nearly the same pancies in literature, it is better to describe the nonlinear processes intensity as 1L-MoS , Fig. 4a. This contrasts ref. , where a pump in LMs using the ratio between the harmonic signal power and the laser at 810 nm was used. We attribute this difference to the fact incident pump power (i.e., harmonic conversion efﬁciency). In this that photons generated in the second-order nonlinear process in case, when comparing the efﬁciencies in our measurements with 49 −10 our set-up with a 1560 nm pump have an energy ~1.6 eV those in ref. , our THG efﬁciency (~4.76 × 10 )is~1.4times 4 NATURE COMMUNICATIONS 8: 893 DOI: 10.1038/s41467-017-00749-4 www.nature.com/naturecommunications | | | THG THG SHG Detected peak power (µW) THG SHG THG peak power (µW) I / I SHG peak power (µW) NATURE COMMUNICATIONS | DOI: 10.1038/s41467-017-00749-4 ARTICLE resonance effects are not observed. In our experiments, the energy THG (pW) of 3ω photons is above the A exciton but does not directly SHG x 37 (pW) overlap with the A or B excitons. Thus, we do not assign the large THG/SHG intensity ratio to an excitonic enhancement, but to the approximate rotational invariance of the 1L-MoS band structure at low energies, which is broken by trigonal warping. SHG is weaker than expected for a non-centrosymmetric material, due to near-isotropic bands contributing to the SHG signal for our low incident photon energies (0.8 eV). Even in the 270 90 presence of a weak trigonal warping, SHG and THG might be comparable above the threshold for two- and three-photon absorption edges. However, this is not a resonant effect. Resonances only emerge when the laser matches a single level (like an excitonic level) rather than a continuum of states . In our analysis, SHG would be absent without trigonal warping. But, trigonal warping alone cannot explain the magnitude of the FHG signal compared to SHG and THG. Figure 4c compares the THG/SHG ratio from experiments and Fig. 5 SHG and THG dependence on the pump light polarization. The polar calculations based on the k·p theory (see Supplementary plot angle corresponds to linearly polarized light when θ = 0° + m·90°, and Note 1) and ﬁnite-temperature diagrammatic perturbation to circularly polarized pump light when θ = 45° + m·90°. The SHG power is theory (see Supplementary Notes 3 and 4). The calculations are multiplied by a factor of 37 to ﬁt in the same scale as THG a factor 2 smaller than the experiments. Considering the com- plexity of the nonlinear optical processes and that our calculations ignore high-energy band structure effects and −10 49 many-body renormalizations , we believe this to be a satisfactory larger than that (~3.38 × 10 )inref. ,while our SHG efﬁciency −11 49 agreement, indicating the importance of trigonal warping in (~6.47 × 10 )istwice that of ref. . Since the effective harmonic generation. susceptibilities are not well deﬁned for LMs and also depend on FHG generally derives from cascades of lower-order nonlinear the calculation method, we believe that the conversion efﬁciency is a multiphoton processes . With an excitation wavelength of better ﬁgure of merit for LMs. 1560 nm, this could be, e.g., a cascade of two SHG processes, where 780 nm photons are ﬁrst generated through SHG Discussion (ω + ω ⇒ ω ) and then undergo another SHG 1560 nm 1560 nm 780 nm Our measurements show that the nonlinear response of 1L-MoS process (ω + ω ⇒ ω ). To yield a FHG at 390 nm 780 nm 780 nm 390 nm and SLG are comparable in magnitude, both revealing stronger of the same intensity as SHG at 780 nm in this cascaded process, nonlinear efﬁciency than three-dimensional nonlinear materials, 1 one would need a conversion efﬁciency (deﬁned as P /P ) 2ω pump 1 59 such as diamond and quartz . This can be explained by for the second SHG process (i.e., ω + ω ⇒ ω )to 780 nm 780 nm 390 nm 27, 34–37, 60 considering their effective Hamiltonians . The main be close to unity. However, we observe a conversion efﬁciency contribution to THG is paramagnetic. This is described by the −10 ~10 for SHG. Therefore, we conclude that our FHG does not square diagram in Supplementary Notes 1–4 (Supplementary arise from cascaded SHGs. Another possible cascade process is Figs. 1–6). This paramagnetic contribution is mainly related to based on THG (ω + ω + ω ⇒ ω ) and 1560 nm 1560 nm 1560 nm 520nm the strong inter-band coupling in the effective Hamiltonian, sum-frequency generation (ω + ω ⇒ ω ). We 520 nm 1560 nm 390 nm c t a 0 0 controlled by large velocity scales, v and v ¼ 300 h ﬁnd that THG strongly increases up to N = 5, as for Fig. 4a. 0:65 ´ for SLG and 1L-MoS , with c the speed of light. The 300 Therefore, we expect this cascaded process to have a similar trend SLG paramagnetic third-harmonic efﬁciency (PTHE) is propor- with N. However, we only observe FHG in 1L-MoS . Thus, we tional to the square of third-order conductivity. Since also exclude this cascade process, and conclude that this is a ð3Þ 2 4 σ / v , we get an overall prefactor v , which explains the (4) yyyy F F direct χ process. strong nonlinear SLG response. Similarly, for 1L-MoS , the We now consider the dependence of our results on the elliptical square diagram contains four paramagnetic current vertices, polarization of the incident light. We consider an incident which gives an overall prefactor v , and an integral over laser beam with arbitrary polarization, i.e., E ¼jj E ε with the dummy momentum variables, which gives a prefactor v ^ε ¼ b x cosðθÞ ± ib y sinðθÞ. Using the crystal symmetries of (see Supplementary Note 3). Therefore, the third-order response 1L-MoS , we derive (see Supplementary Note 2) the following ð3Þ (2) function, Π , is proportional to v , which implies a scaling expressions for the second- and third-order polarizations P yyyy 4 (3) of PTHE as v . Exciton physics is not considered because our and P : experimental conditions only capture off-resonance transitions. ð2Þ ð2Þ 2 1L-MoS is transparent at this wavelength due to its ~1.9 eV P ¼ ϵ χ jj E½ i sinð2θÞb x b y ð3Þ yyy 12 61 gap , while SLG absorbs 2.3% of the light . Therefore, 1L-MoS and other TMDs are promising for integration with waveguides and or ﬁbers for all-optical nonlinear devices, such as all-optical modulators and signal processing devices, where materials with ð3Þ ð3Þ 3 P ¼ ϵ χ jj E ^ε cosð2θÞ: ð4Þ 0 ± yyyy nonlinear properties are essential . TheSHG andTHG powerdependencefollows quadraticand cubic trends, Fig. 4b. At our power levels, THG is up to 30 times Note that θ = 0° corresponds to a linearly polarized laser along stronger than SHG. 1L-TMDs have strongly bound excitons that the b x direction, perpendicular to the D mirror symmetry plane, 3h 62–64 can modify their optical properties . The exciton resonances while θ = 45° corresponds to a circularly polarized laser. From 17, 65, 66 51, 55 also affect their nonlinear optical responses . References Eq. (3), we expect the intensity of SHG in response to a circularly reported that when the SHG energy is above the A and B excitons, polarized pump laser to be twice that of a linearly polarized laser. NATURE COMMUNICATIONS 8: 893 DOI: 10.1038/s41467-017-00749-4 www.nature.com/naturecommunications 5 | | | ARTICLE NATURE COMMUNICATIONS | DOI: 10.1038/s41467-017-00749-4 a bc SHG THG 1L 7L 2L 6L 3L 4L 5L 20 µm Fig. 6 Optical and multiphoton images of few-layer MoS ﬂake. a Optical micrograph, b SHG, and c THG images of ﬂake with few-layer areas under 1560 nm excitation pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ (3) ð1Þ χ (−3ω;ω, ω, ω) is the third-order optical susceptibility, n ¼ ϵ ðjωÞ, with j¼1;3 Equation (4) implies vanishing THG in response to a circularly ð1Þ ϵ the TMD linear dielectric function. Δkt is the phase mismatch between the polarized pump laser. fundamental and third harmonic generated waves. We measure the dependence of SHG and THG on elliptical For Δkt ≈ 0, THG adds up quadratically with light propagation length (i.e., t ∝ polarization using a linearly polarized laser and a rotating QWP. N). The signal starts to saturate for N = 6. The possible reasons for subquadratic signal build-up can be either phase mismatch, or absorption . For THG, Δk = Depending on the angle θ between the QWP axes and the laser 3k ± k , where k and k are the wavevectors of the incident and THG signals, in 3ω in 3ω polarization, the excitation light is linearly (θ = 0° + m·90°) or respectively, where the plus sign indicates THG generated in the backward circularly (θ = 45° + m·90°) polarized. Figure 5 shows that the direction, while minus identiﬁes forward generated THG. Even for backward experimental data are in agreement with Eqs. (3) and (4). generated THG, Δkt ≈ 0 for 6L-MoS (~4.3 nm ). This rules out phase mismatch as the origin of the signal saturation when N ≤ 6. Therefore, we assume that the The THG signal is maximum for a linearly polarized excitation signal saturation is due to absorption of the third harmonic light. laser, while it vanishes for circularly polarized light. SHG is always visible, but its intensity is maximum for circularly polarized light. Diagrammatic nonlinear response theory. To quantify theoretically the strength Given that harmonic generation is strongly dependent on the of nonlinear harmonic generation processes, we generalize the diagrammatic perturbation theory approach to the case of TMDs. We combine this technique symmetry and stacking of layers and that different 1L-TMDs 11, 14, 15, 21 with a low-energy k·p model Hamiltonian HðÞ k for 1L-MoS . In such low-energy (e.g., WSe , MoSe ) all have similar nonlinear response , 2 2 35, 39 model, light-matter interactions are treated by employing minimal coupling , one could use heterostructures (e.g., MoS /WSe ) to engineer 2 2 k → k + eA(t)/ħ, where A(t) is a time-dependent uniform vector potential. SHG and other nonlinear processes for high photon-conversion Nonlinear response functions are calculated via the multi-legged Feynman diagrams depicted in Supplementary Figs. 2 and 3. efﬁciency for a wide range of applications requiring the genera- tion of higher frequencies. This may lead to the use of LMs and heterostructures for applications utilizing optical nonlinearities Data availability. The data that support the ﬁndings of this study are available (e.g., all-optical devices, frequency combs, high-order harmonic from the corresponding author on request. generation, multiphoton microscopy, and therapy etc.). Received: 8 November 2016 Accepted: 26 July 2017 Methods Determination of MoS thickness from SHG and THG signals. SHG and THG for FL-MoS (N = 1…7) are studied on the ﬂakes in Fig. 6a. SHG and THG images are shown in Fig. 6b, c. At 1560 nm, the contrast between 1 and 3L areas is small, as well as the contrast between 3, 5, and 7 L regions (Fig. 6b). The THG signal increases up to N = 7, Figs. 4a and 6c. On the other hand, the SHG signal (Fig. 6b) is only generated in ON ﬂakes, due to symmetry . Therefore, References areas with intensity between the 3, 5, and 7L regions in Fig. 6c, but dark in SHG, 1. Boyd, R. W. Nonlinear Optics (Academic Press, 2003). are 4 and 6 L. The dependence of the intensities of THG and SHG on N is plotted 2. Pavone, F. S. & Campagnola, P. J. Second Harmonic Generation Imaging in Fig. 4a. The combination of SHG and THG can be used to identify N at least up (Taylor & Francis, 2013). to 7. The THG signal develops as a function of N. Using Maxwell’s equations for a 3. Saleh, B. E. A. & Teich, M. C. Fundamentals of Photonics (Academic Press, nonlinear medium with thickness t and considering the slowly varying amplitude 2003). 1, 69 approximation , we obtain: 4. Willner, A. E., Khaleghi, S., Chitgarha, M. R. & Yilmaz, O. F. All-optical signal processing. J. Lightwave Technol 32, 660–680 (2014). I ð3ωÞ I 2 Δkt 3ω in ð3Þ 2 2 5. Zipfel, W. R., Williams, R. M. & Webb, W. W. Nonlinear magic: multiphoton χ ð3ω; ω; ω; ωÞ t sinc ; ð5Þ 3 2 4 I 16n n ϵ c 2 in 1 3 0 microscopy in the biosciences. Nat. Biotechnol. 21, 1369–1377 (2003). 6. Bhawalkar, J. D., He, G. S. & Prasad, P. N. Nonlinear multiphoton processes in where I and I are the intensities of the incident and THG light, respectively, and organic and polymeric materials. Rep. Prog. Phys. 59, 1041 (1996). in 3ω 6 NATURE COMMUNICATIONS 8: 893 DOI: 10.1038/s41467-017-00749-4 www.nature.com/naturecommunications | | | Intensity (a.u.) Intensity (a.u.) NATURE COMMUNICATIONS | DOI: 10.1038/s41467-017-00749-4 ARTICLE 7. Tsang, T. Y. F. Optical third-harmonic generation at interfaces. Phys. Rev. A 52, 40. Bonaccorso, F. et al. Production and processing of graphene and 2d crystals. 4116 (1995). Mater. Today 15, 564–589 (2012). 8. Karvonen, L. et al. Investigation of second-and third-harmonic generation in 41. Sundaram, R. et al. Electroluminescence in single layer MoS . Nano Lett. 13, few-layer gallium selenide by multiphoton microscopy. Sci. Rep. 5, 10334 1416–1421 (2013). 42. Casiraghi, C. et al. Rayleigh imaging of graphene and graphene layers. Nano (2015). Lett. 7, 2711–7 (2007). 9. Bonaccorso, F., Sun, Z., Hasan, T. & Ferrari, A. C. Graphene photonics and 43. Zhang, X. et al. Raman spectroscopy of shear and layer breathing modes in optoelectronics. Nat. Photon 4, 611–622 (2010). 10. Ferrari, A. C. et al. Science and technology roadmap for graphene, related multilayer MoS . Phys. Rev. B 87, 115413 (2013). 44. Säynätjoki, A. et al. Rapid large-area multiphoton microscopy for two-dimensional crystals, and hybrid systems. Nanoscale 7, 4598–4810 (2015). characterization of graphene. ACS Nano 7, 8441–8446 (2013). 11. Sun, Z., Martinez, A. & Wang, F. Optical modulators with 2D layered materials. 45. Kieu, K., Jones, R. J. & Peyghambarian, N. Generation of few-cycle pulses from Nat. Photon. 10, 227–238 (2016). 12. Mak, K. F., Lee, C., Hone, J., Shan, J. & Heinz, T. F. Atomically thin MoS :a an ampliﬁed carbon nanotube mode-locked ﬁber laser system. IEEE Photon. new direct-gap semiconductor. Phys. Rev. Lett. 105, 136805 (2010). Technol. Lett. 22, 1521–1523 (2010). 46. Kieu, K., Jones, R. J. & Peyghambarian, N. High power femtosecond source 13. Eda, G. et al. Photoluminescence from chemically exfoliated MoS . Nano Lett. near 1 micron based on an all-ﬁber er-doped mode-locked laser. Opt. Express 11, 5111–5116 (2011). 18, 21350–21355 (2010). 14. Li, Y. et al. Probing symmetry properties of few-layer MoS and h-BN by 47. Miller, R. C. Optical second harmonic generation in piezoelectric crystals. Appl. optical second-harmonic generation. Nano Lett. 13, 3329–3333 (2013). Phys. Lett. 5,17–19 (1964). 15. Kumar, N. et al. Second harmonic microscopy of monolayer MoS . Phys. Rev. B 48. Chin, A. H., Calderón, O. G. & Kono, J. Extreme midinfrared nonlinear optics 87, 161403 (2013). in semiconductors. Phys. Rev. Lett. 86, 3292 (2001). 16. Wang, K. et al. Ultrafast saturable absorption of two-dimensional MoS 49. Woodward, R. I. et al. Characterization of the second- and third-order nanosheets. ACS Nano 7, 9260–9267 (2013). nonlinear optical susceptibilities of monolayer MoS using multiphoton 17. Malard, L. M., Alencar, T. V., Barboza, A. P. M., Mak, K. F. & de Paula, A. M. 2 microscopy. 2D Mater 4, 011006 (2017). Observation of intense second harmonic generation from MoS atomic crystals. 50. Säynätjoki, A. et al. Ultra-strong nonlinear optical processes and Phys. Rev. B 87, 201401 (2013). trigonal warping in MoS layers. Preprint at https://arxiv.org/abs/1608.04101 18. Wang, R. et al. Third-harmonic generation in ultrathin ﬁlms of MoS . ACS 2 (2016). Appl. Mater. Interfaces 6, 314–318 (2013). 51. Clark, D. et al. Near bandgap second-order nonlinear optical characteristics of 19. Trolle, M. L., Seifert, G. & Pedersen, T. G. Theory of excitonic second-harmonic MoS monolayer transferred on transparent substrates. Appl. Phys. Lett. 107, generation in monolayer MoS . Phys. Rev. B 89, 235410 (2014). 131113 (2015). 20. Clark, D. et al. Strong optical nonlinearity of CVD-grown MoS monolayer as 52. Le, C. T. et al. Impact of selenium doping on resonant second harmonic probed by wavelength-dependent second-harmonic generation. Phys. Rev. B 90, generation in monolayer MoS . ACS Photon. 4,38–44 (2017). 121409 (2014). 2 53. Liu, H. et al. High-harmonic generation from an atomically thin 21. Seyler, K. L. et al. Electrical control of second-harmonic generation in a WSe semiconductor. Nat. Phys 13, 262–265 (2017). monolayer transistor. Nat. Nanotechnol 10, 407–411 (2015). 54. Janisch, C. et al. Extraordinary second harmonic generation in tungsten 22. Kuc, A., Zibouche, N. & Heine, T. Inﬂuence of quantum conﬁnement on the disulﬁde monolayers. Sci. Rep. 4, 5530 (2014). electronic structure of the transition metal sulﬁde TS . Phys. Rev. B 83, 245213 55. Le, C. T. et al. Nonlinear optical characteristics of monolayer MoSe . Ann. Phys (2011). 528, 551–559 (2016). 23. Kadantsev, E. S. & Hawrylak, P. Electronic structure of a single MoS 56. Kumar, N. et al. Third harmonic generation in graphene and few-layer graphite monolayer. Solid State Commun 152, 909–913 (2012). ﬁlms. Phys. Rev. B 87, 121406 (2013). 24. Wang, Q. H., Kalantar-Zadeh, K., Kis, A., Coleman, J. N. & Strano, M. S. 57. Hendry, E., Hale, P. J., Moger, J., Savchenko, A. & Mikhailov, S. Coherent Electronics and optoelectronics of two-dimensional transition metal nonlinear optical response of graphene. Phys. Rev. Lett. 105, 097401 (2010). dichalcogenides. Nat. Nanotechnol 7, 699–712 (2012). 58. Cheng, J., Vermeulen, N. & Sipe, J. Third order optical nonlinearity of 25. Shi, H., Pan, H., Zhang, Y.-W. & Yakobson, B. I. Quasiparticle band structures graphene. New J. Phys. 16, 053014 (2014). and optical properties of strained monolayer MoS and WS . Phys. Rev. B 87, 2 2 59. Hong, S.-Y. et al. Optical third-harmonic generation in graphene. Phys. Rev. X 155304 (2013). 3, 021014 (2013). 26. Zahid, F., Liu, L., Zhu, Y., Wang, J. & Guo, H. A generic tight-binding model 60. Neto, A. H. C., Guinea, F., Peres, N. M., Novoselov, K. S. & Geim, A. K. The for monolayer, bilayer and bulk MoS . AIP Adv. 3, 052111 (2013). electronic properties of graphene. Rev. Mod. Phys. 81, 109 (2009). 27. Kormányos, A. et al. Monolayer MoS : trigonal warping, the γ valley, and 61. Nair, R. R. et al. Fine structure constant deﬁnes visual transparency of spin-orbit coupling effects. Phys. Rev. B 88, 045416 (2013). graphene. Science 320, 1308–1308 (2008). 28. Qiu, D. Y., Felipe, H. & Louie, S. G. Optical spectrum of MoS : many-body 62. Ramasubramaniam, A. Large excitonic effects in monolayers of molybdenum effects and diversity of exciton states. Phys. Rev. Lett. 111, 216805 (2013). and tungsten dichalcogenides. Phys. Rev. B 86, 115409 (2012). 29. Gibertini, M., Pellegrino, F. M., Marzari, N. & Polini, M. Spin-resolved optical 63. Cheiwchanchamnangij, T. & Lambrecht, W. R. L. Quasiparticle band structure conductivity of two-dimensional group-VIb transition-metal dichalcogenides. calculation of monolayer, bilayer, and bulk MoS . Phys. Rev. B 85, 205302 (2012). Phys. Rev. B 90, 245411 (2014). 64. Mak, K. F. et al. Tightly bound trions in monolayer MoS . Nat. Mater. 12, 30. Margulis, V. A., Muryumin, E. E. & Gaiduk, E. A. Optical second-harmonic 207–211 (2013). generation from two-dimensional hexagonal crystals with broken space 65. Grüning, M. & Attaccalite, C. Second harmonic generation in h-BN and inversion symmetry. J. Phys. Condens. Matter 25, 195302 (2013). MoS monolayers: role of electron-hole interaction. Phys. Rev. B 89, 081102 31. Wu, S. et al. Quantum-enhanced tunable second-order optical nonlinearity in (2014). bilayer graphene. Nano Lett. 12, 2032–2036 (2012). 66. Wang, G. et al. Giant enhancement of the optical second-harmonic emission of 32. Brun, S. J. & Pedersen, T. G. Intense and tunable second-harmonic generation WSe monolayers by laser excitation at exciton resonances. Phys. Rev. Lett. 114, in biased bilayer graphene. Phys. Rev. B 91, 205405 (2015). 097403 (2015). 33. Hipolito, F., Pedersen, T. G. & Pereira, V. M. Nonlinear photocurrents in 67. Haug, H. & Koch, S. W. Quantum Theory of the Optical and Electronic two-dimensional systems based on graphene and boron nitride. Phys. Rev. B 94, Properties of Semiconductors (World Scientiﬁc Publishing, 2009). 045434 (2016). 68. Zhu, S.-n, Zhu, Y.-y & Ming, N.-b Quasi-phase-matched third-harmonic 34. Xiao, D., Liu, G.-B., Feng, W., Xu, X. & Yao, W. Coupled spin and valley generation in a quasi-periodic optical superlattice. Science 278, 843–846 physics in monolayers of MoX and other group-vi dichalcogenides. Phys. Rev. (1997). Lett. 108, 196802 (2012). 69. Butcher, P. N. & Cotter, D. The Elements of Nonlinear Optics (Cambrige 35. Rostami, H., Roldán, R., Cappelluti, E., Asgari, R. & Guinea, F. Theory of University Press, 1990). strain in single-layer transition metal dichalcogenides. Phys. Rev. B 92, 195402 70. Radisavljevic, B., Radenovic, A., Brivio, J., Giacometti, I. V. & Kis, A. Single- (2015). layer MoS transistors. Nat. Nanotechnol 6, 147–150 (2011). 36. Rostami, H., Asgari, R. & Guinea, F. Edge modes in zigzag and armchair ribbons of monolayer MoS . J. Phys. Condens. Matter 28, 495001 (2016). 37. Rostami, H., Moghaddam, A. G. & Asgari, R. Effective lattice hamiltonian for monolayer MoS : tailoring electronic structure with perpendicular electric and 2 Acknowledgements magnetic ﬁelds. Phys. Rev. B 88, 085440 (2013). We thank M.J. Huttunen and R.W. Boyd for useful discussions. We acknowledge funding 38. Alidoust, N. et al. Observation of monolayer valence band spin-orbit effect and from the Academy of Finland (Nos: 276376, 284548, 295777, 298297, and 304666), induced quantum well states in MoX . Nat. Commun 5, 4673 (2014). TEKES (NP-Nano, OPEC), Royal Academy of Engineering (RAEng) Research Fellow- 39. Rostami, H. & Polini, M. Theory of third-harmonic generation in graphene: a ships, Fondazione Istituto Italiano di Tecnologia, the Graphene Flagship, ERC grants diagrammatic approach. Phys. Rev. B 93, 161411 (2016). Hetero2D, Nokia Foundation, EPSRC Grants EP/K01711X/1, EP/K017144/1, EP/ NATURE COMMUNICATIONS 8: 893 DOI: 10.1038/s41467-017-00749-4 www.nature.com/naturecommunications 7 | | | ARTICLE NATURE COMMUNICATIONS | DOI: 10.1038/s41467-017-00749-4 L016087/1, AFOSR COMAS MURI (FA9550-10-1-0558), ONR NECom MURI, CIAN Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in NSF ERC under Grant EEC-0812072, and TRIF Photonics funding from the state of published maps and institutional afﬁliations. Arizona and the Micronova, Nanofabrication Centre of Aalto University. Open Access This article is licensed under a Creative Commons Author contributions Attribution 4.0 International License, which permits use, sharing, A.S., L.K., A.A., S.M., K.K., and Z.S. carried out the multiphoton experiments and data adaptation, distribution and reproduction in any medium or format, as long as you give analysis. Samples preparation and characterization were carried out by A.L. and A.C.F. appropriate credit to the original author(s) and the source, provide a link to the Creative The nonlinear response function calculations were carried out by H.R. and M.P. Sample Commons license, and indicate if changes were made. The images or other third party fabrication, multiphoton characterization, and analysis were coordinated by R.A.N., N.P., material in this article are included in the article’s Creative Commons license, unless H.L., A.C.F., M.P., and Z.S. All authors contributed to the manuscript. indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory Additional information regulation or exceeds the permitted use, you will need to obtain permission directly from Supplementary Information accompanies this paper at 10.1038/s41467-017-00749-4. the copyright holder. To view a copy of this license, visit http://creativecommons.org/ licenses/by/4.0/. Competing interests: The authors declare no competing ﬁnancial interests. Reprints and permission information is available online at http://npg.nature.com/ © The Author(s) 2017 reprintsandpermissions/ 8 NATURE COMMUNICATIONS 8: 893 DOI: 10.1038/s41467-017-00749-4 www.nature.com/naturecommunications | | |
Nature Communications – Springer Journals
Published: Oct 12, 2017
You can share this free article with as many people as you like with the url below! We hope you enjoy this feature!
Read and print from thousands of top scholarly journals.
Already have an account? Log in
Bookmark this article. You can see your Bookmarks on your DeepDyve Library.
To save an article, log in first, or sign up for a DeepDyve account if you don’t already have one.
Copy and paste the desired citation format or use the link below to download a file formatted for EndNote
Access the full text.
Sign up today, get DeepDyve free for 14 days.
All DeepDyve websites use cookies to improve your online experience. They were placed on your computer when you launched this website. You can change your cookie settings through your browser.